A maior rede de estudos do Brasil

Grátis
81 pág.

## Pré-visualização | Página 2 de 12

```nm
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.

3-10
3.9 This problem asks for us to calculate the radius of a tantalum atom. For BCC, n = 2 atoms/unit cell,
and

VC =
4 R
3
⎛
⎝
⎜
⎞
⎠
⎟
3
= 64 R
3
3 3

Since, from Equation 3.5

ρ =
nATa
VC N A

=
nATa
64 R3
3 3
⎛
⎝
⎜ ⎜
⎞
⎠
⎟ ⎟ N A

and solving for R the previous equation

R =
3 3nATa
64ρ N A
⎛
⎝
⎜ ⎜
⎞
⎠
⎟ ⎟
1/3

= (3 3) (2 atoms/unit cell) (180.9 g/mol)
(64)(16.6 g/cm3)(6.023 x 1023 atoms/mol)
⎡
⎣
⎢
⎢
⎤
⎦
⎥
⎥
1/3

= 1.43 x 10-8 cm = 0.143 nm
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.

3-11
3.10 For the simple cubic crystal structure, the value of n in Equation 3.5 is unity since there is only a
single atom associated with each unit cell. Furthermore, for the unit cell edge length, a = 2R (Figure 3.23).
Therefore, employment of Equation 3.5 yields

ρ = nA
VC N A
= nA
(2 R)3 N A

= (1 atom/unit cell)(74.5 g/mol)
(2)(1.45 x 10-8 cm)
⎡
⎣
⎢
⎤
⎦
⎥
3
/(unit cell)
⎧
⎨
⎪
⎩ ⎪
⎫
⎬
⎪
⎭ ⎪
(6.023 x 1023 atoms/mol)

5.07 g/cm3
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.

3-12
3.11 (a) The volume of the Ti unit cell may be computed using Equation 3.5 as

VC =
nATi
ρN A

Now, for HCP, n = 6 atoms/unit cell, and for Ti, ATi = 47.9 g/mol. Thus,

VC =
(6 atoms/unit cell)(47.9 g/mol)
(4.51 g/cm3)(6.023 x 1023 atoms/mol)

= 1.058 x 10-22 cm3/unit cell = 1.058 x 10-28 m3/unit cell

(b) From part of the solution to Problem 3.6, for HCP

VC = 6 R
2c 3

But, since a = 2R, (i.e., R = a/2) then

VC = 6
a
2
⎛
⎝
⎜
⎞
⎠
⎟
2
c 3 =
3 3 a2c
2

but, since c = 1.58a

VC =
3 3 (1.58) a3
2
= 1.058 x 10-22 cm3/unit cell

Now, solving for a

a = (2)(1.058 x 10
-22 cm3)
(3)( 3) (1.58)
⎡
⎣
⎢
⎢
⎤
⎦
⎥
⎥
1/3

= 2.96 x 10-8 cm = 0.296 nm

And finally
c = 1.58a = (1.58)(0.296 nm) = 0.468 nm
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.

3-13
3.12 This problem asks that we calculate the theoretical densities of Al, Ni, Mg, and W.
Since Al has an FCC crystal structure, n = 4, and VC = 16R
3 2 (Equation 3.4). Also, R = 0.143 nm (1.43
x 10-8 cm) and AAl = 26.98 g/mol. Employment of Equation 3.5 yields

ρ =
nAAl
VC N A

= (4 atoms/unit cell)(26.98 g/mol)
(2)(1.43 x 10-8 cm)( 2)[ ]3/(unit cell)⎧ ⎨
⎩
⎫
⎬
⎭
(6.023 x 1023 atoms/mol)

= 2.71 g/cm3

The value given in the table inside the front cover is 2.71 g/cm3.
Nickel also has an FCC crystal structure and therefore

ρ = (4 atoms/unit cell)(58.69 g/mol)
(2)(1.25 x 10-8 cm)( 2)[ ]3/(unit cell )⎧ ⎨
⎩
⎫
⎬
⎭
(6.023 x 1023 atoms/mol)

= 8.82 g/cm3

The value given in the table is 8.90 g/cm3.

Magnesium has an HCP crystal structure, and from the solution to Problem 3.6,

VC =
3 3 a2c
2

and, since c = 1.624a and a = 2R = 2(1.60 x 10-8 cm) = 3.20 x 10-8 cm

VC =
(3 3)(1.624)(3.20 x 10-8 cm)3
2
= 1.38 x 10−22 cm3/unit cell

Also, there are 6 atoms/unit cell for HCP. Therefore the theoretical density is

ρ =
nAMg
VC N A

Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.

3-14

= (6 atoms/unit cell)(24.31 g/mol)
(1.38 x 10-22 cm3/unit cell)(6.023 x 1023 atoms/mol)

= 1.75 g/cm3

The value given in the table is 1.74 g/cm3.

Tungsten has a BCC crystal structure for which n = 2 and a =

4 R
3
(Equation 3.3); also AW = 183.85
g/mol and R = 0.137 nm. Therefore, employment of Equation 3.5 leads to

ρ = (2 atoms/unit cell)(183.85 g/mol)
(4)(1.37 x 10-8 cm)
3
⎡
⎣
⎢
⎢
⎤
⎦
⎥
⎥
3
/(unit cell)
⎧
⎨
⎪
⎩ ⎪
⎫
⎬
⎪
⎭ ⎪
(6.023 x 1023 atoms/mol)

= 19.3 g/cm3

The value given in the table is 19.3 g/cm3.
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.

3-15
3.13 In order to determine whether Nb has an FCC or a BCC crystal structure, we need to compute its
density for each of the crystal structures. For FCC, n = 4, and a = 2 R 2 (Equation 3.1). Also, from Figure 2.6, its
atomic weight is 92.91 g/mol. Thus, for FCC (employing Equation 3.5)

ρ =
nANb
a3N A
=
nANb
(2R 2)3N A

= (4 atoms/unit cell)(92.91 g/mol)
(2)(1.43 × 10-8 cm)( 2)[ ]3 /(unit cell)⎧ ⎨
⎩
⎫
⎬
⎭
(6.023 × 1023 atoms /mol)

= 9.33 g/cm3

For BCC, n = 2, and a =

4 R
3
(Equation 3.3), thus

ρ =
nANb
4 R
3
⎛
⎝
⎜ ⎜
⎞
⎠
⎟ ⎟
3
N A

ρ = (2 atoms/unit cell)(92.91 g/mol)
(4)(1.43 × 10-8 cm)
3
⎡
⎣
⎢
⎢
⎤
⎦
⎥
⎥
3
/(unit cell)
⎧
⎨
⎪
⎩ ⎪
⎫
⎬
⎪
⎭ ⎪
(6.023 × 1023 atoms /mol)

= 8.57 g/cm3

which is the value provided in the problem statement. Therefore, Nb has a BCC crystal structure.
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled in courses for which the textbook has been adopted. Any other reproduction or translation of this work beyond that permitted
by Sections 107 or 108 of the 1976 United States Copyright Act without the permission of the copyright owner is unlawful.

3-17

ρ =
nAC
4R
3
⎛
⎝
⎜
⎞
⎠
⎟
3
N A

= (2 atoms/unit cell)(91.6 g/mol)
(4)(1.37 × 10-8 cm)
3
⎡
⎣
⎢
⎢
⎤
⎦
⎥
⎥
3
/(unit cell)
⎧
⎨
⎪
⎩ ⎪
⎫
⎬
⎪
⎭ ⎪
(6.023 × 1023 atoms/mol)

= 9.60 g/cm3
Therefore, its crystal structure is BCC.
Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to
students enrolled```